# Nanocomposite Materials of Alternately StackedC60 Monolayer and Graphene

Authors: Makoto Ishikawa; Shu Kamiya; Shoji Yoshimoto; Masaru Suzuki; Daisuke Kuwahara; Naruo Sasaki; Kouji Miura
Journal: Journal of Nanomaterials
 (2010)

---

## Abstract

We synthesized the novel nanocomposite consisting alternately of a stacked single graphene sheet and aC60 monolayer by using the graphite intercalation technique in which alkylamine molecules help intercalate large C60 molecules into the graphite. Moreover, it is found that the intercalated C60 molecules can rotate in between single graphene sheets by using C13 NMR measurements. This preparation method provides a general way for intercalating huge fullerene molecules into graphite, which will lead to promising materials with novel mechanical, physical, and electrical properties.


---

## Body

## 1. Introduction

C60 intercalated graphite has previously been designed, and the electronic properties and stabilities have been studied theoretically [1]. It is also reported that the C60 intercalated graphite may possess potential applications in semiconductor [2] and hydrogen storage device [3]. On the other hand, fullerene molecules, especially, C60, also have unique lubrication effects, and they have been treated as a lubricant due to their spherical shape [4–6]. Up to now, we have studied C60 monolayers confined by graphite flakes [7] and C60 monolayers included among graphite [8–10], which, interestingly, exhibit ultralow friction, because quasi-freely rotating C60 molecules act as molecular bearings. However, it is quite difficult to perform a mass production for intercalating C60 molecules into graphite and to provide nanomaterials with a perfectly alternate stacking of C60 monolayer and graphene in previous studies.Here we show nanocomposite materials consisting alternately of a stacked single graphene sheet, by the graphite intercalation technique in which alkylamine molecules help intercalate largeC60 molecules into the graphite.


## 2. Experimental

First, graphite oxide (GO) was synthesized from graphite powder with an average size of 500μm (Nippon Carbon Co., Ltd.) in accordance with the Hummers method [12] with some modifications, and the intercalation of octylamine into graphite (GO-OA) was performed as described previously in [13, 14]. Next, octylamine-intercalated graphite oxide (GO-OA) was added to fullerene solution (100 mg of C60 dissolved in 100 mL toluene), and after that, the toluene used was evaporated at room temperature, leaving behind in the products (GO-OA-C60). The C60 fullerene used in this experiment was purchased from Frontier Carbon Co., Ltd, in Japan. The products of GO-OA-C60 were treated with 0.1 N hydrochloric acid solution at room temperature for at least 30 minutes and dried in air at 80°C overnight to remove the octylamine, resulting in the C60-intercalated graphite oxide (GO-C60). Finally, in order to remove C60 powders that are not intercalated into the graphite, and moreover, to remove octylamines that are intercalated into the graphite, GO-C60 was heated for at least 80 minutes at 600°C under a high vacuum of 10-6 Torr, which results in the nanocomposite consisting alternately of a stacked single graphene sheet and a C60 monolayer. All specimens were analyzed by using X-ray diffraction (Rigaku RINT 2200/PC diffractometer: CuKα radiation at 40 kV and 30 mA), FT-IR spectroscopy (FTIR: JASCO 480 Plus FT-IR spectrometer: the samples in KBr pellets), NMR (our original 7.1 T spectrometer with a Tecmag Apollo spectrometer and a Doty SuperSonic MAS 7 mm probe head), and high-resolution electron microscopy (JEM3100FEF: a lattice resolution of 0.1 nm when it is operated at an acceleration voltage of 300 kV).


## 3. Results and Discussion

Figure1(a) shows the X-ray diffraction (XRD) intensity from graphite oxide (GO) and alkylamine-intercalated graphite oxide (GO-amine) with different alkyl chain lengths (CnH2n+1NH2) (n=3 to 8). The appearance of a peak in the GO of Figure 1(a) shows that the spacing between graphite oxide sheets is approximately 8 Å, which is identical to the published data [12]. It is found that the spacing between graphite oxide sheets in the case of the GO-amine (n=3 to 8) increases with the increase in the length of the alkyl chain incorporated in the interlayer space of the GO. Figure 1(b) shows the XRD intensity from the GO-amine (n=3 to 8) in C60 solution, which we call the C60-intercalated graphite oxide (GO-C60). It should be noted that there appear drastic changes in the XRD intensity between n=5 and n=6 in Figure 1(b), which indicates that C60 molecules are intercalated in the interlayer space of the GO by the driving force of alkylamine situated at between the graphene oxide sheets when the interlayer space is sufficiently larger than the C60 molecule. However, there exist many C60 powders which are not intercalated into the GO in these GO-C60 specimens because the stronger peaks, (111),(220),(311),(222),(331),(420),(422), and (511), of XRD intensity from C60 powders (JCPDS file No.44-0558) appear in the spectra of Figure 1(b). In order to remove C60 powders that are not intercalated into the GO, and moreover, to expel the alkylamines which are intercalated into the graphite, the GO-C60 specimens of Figure 1(b) were heated for 80 minutes at 600°C under a high vacuum of 10-6 Torr, as shown in Figure 2. It should be noted that n=6,n=7, and n=8 have broad peaks of A and B corresponding to d-spacings of 9 Å and 4.6 Å, respectively, in addition to a broad peak of d=3.3Å corresponding to the spacing of graphite layers, although n=3,n=4, and n=5 have only a single broad peak of d=3.3Å. Since the GO-amine reverts to the graphite layers when alkylamines leaves the GO-amine host after heating at up to 600°C, as shown in the XRD intensity of Figure 3, the graphene oxide layers in the GO-C60, which do not include C60 molecules, also revert to the graphite layers when alkylamines go out from it after heating. It is expected that the peaks of A and B (n=6 to 8) in Figure 2 are due to the d-spacing between the graphenes intercalating the C60 monolayer and their stacking faults (the disorder of the stacking) [15], respectively. However, since peak A is also widely distributed, the d-spacings between the graphenes intercalating the C60 monolayer are considered to be widely distributed.XRD intensity from as-prepared samples. (a) XRD intensity from graphite oxide (GO) and alkylamine-intercalated graphite oxides (GO-amine) with different chain lengths(CnH2n+1NH2)(n=3–8). The peaks of GO and GO-amine are indicated by the arrows in the figure. (b) XRD intensity from GO-amine with different chain lengths in C60 solution (n=3–8).
(a)(b)Figure 2
XRD intensity from the specimens heated for 80 minutes at600°C under a high vacuum of 10-6 Torr for the GO-C60 specimens of Figure 1(b).Figure 3
XRD intensity from the specimens heated for 80 minutes at600°C under high vacuum of 10-6 Torr for alkylamine-intercalated graphite oxide (GO-amine).Figure4 shows the FT-IR spectra from the specimens of Figure 2. This result is consistent with the conclusion based on Figure 2 that C60 molecules can be intercalated into the GO with alkylamine chains longer than that of n=5 because the FT-IR spectra from n=6,n=7, and n=8 in Figure 4 exhibit the C60 intermolecular IR-active (F1u) modes [11] although those with the shorter alkylamine chains do not exhibit these modes. However, one mode of 526 cm-1 among IR-active (F1u) modes only appears in these FT-IR spectra because the number of C60 molecules included in the specimens is rather small.Figure 4
FT-IR spectra from the specimens of Figure2. The C60 intermolecular IR-active (F1u) modes are indicated in the inset of the figure.The rotational dynamics ofC60 molecules between graphenes have been investigated by 13C NMR in the temperature range from room temperature to -80°C. We prepared C60 materials 20–30% enriched in 13C in order to increase the 13C NMR signal. The present specimen was mixed with Na2SO4 in a weight ratio of 1 : 50 to avoid arcing in a NMR probe. The NMR experiments were performed at 75.4 MHz for 13C in an external field of 7.1 T by the pulse inversion recovery method. 13C NMR spectra were taken by Fourier transforming the signal following the π/2 pulse. The typical π/2 pulse width was 5.4 us. It is well known that for C60 molecules in solid C60 at room temperature, large rotational motion averages out the chemical-shift anisotropy (CSA) and the 13C NMR spectra show motional narrowing of 2.5 ppm in width. In contrast, spectra broaden at low temperature and develop the CSA power pattern with a CSA tensor with the principle values δ11=213ppm,δ22=182ppm, and δ33=33ppm [11]. Figure 5 shows the 13C NMR spectra for the specimens of Figure 2 at room temperature, where the 13C NMR spectrum at room temperature is the same as that at the temperature of -80°C. Only one sharp line with a peak position of 144 ppm was observed, and its line shape is a Gaussian-like function with an FWHM value of 5 ppm. The positions are in good agreement with the average principle values for C60 molecules in solid C60, and the linewidth is about one-twentieth narrower than that of the powder pattern [11]. These observations clearly demonstrate the lack of the polymerization [16] of C60 molecules in the present material. Furthermore, the observed Gaussian-like line shape means a motional narrowing and that C60 molecules rotate quasi-freely with a correlation time on the order of 10 ps. This correction time is similar to that of the same case [17]. This means that no strong bonding such as chemical bonding between the graphenes and C60 molecules is made, and C60 molecules easily rotate for outer force.Figure 5
The13C NMR spectra for the specimens of Figure 2 at room temperature. Only one sharp line with a peak position of 144 ppm [11] was observed.It is possible that the specimens in the case of Figure2 are broken into nanoribbons of nanometer thickness by ultrasonic vibration, which is analogous to the preparation method of the graphene nanoribbon. A high-resolution electron microscope (HR-TEM) image of the nanoribbon is shown in Figure 6(a). First, two parts of graphene layers (areas A) are shown in Figure 6(a). A missing rows of zigzag chains clearly appear in the graphene network, which indicates that the thickness of the specimen is on an atomic scale [18], and moreover, moire patterns formed by graphenes also appear in area A. It is expected that the contrast of area B originates from the C60 molecules confined between graphene sheets, although we will discuss this contrast later in detail. Now we illustrate the structure model of C60-intercalated graphite in Figure 6(b), that is, the nanocomposite consisting of alternately stacked graphene sheets and C60 monolayers in which C60 molecules can form a monolayer and rotate between graphene sheets.High-resolution electron microscope (HR-TEM) image and structure model of alternately stacked graphene sheets andC60 monolayers. (a) High-resolution electron microscope (HR-TEM) image from the nanoribbon of the specimens of Figure 2. Graphene layers (area: A) and C60 molecules between graphene sheets (area: B) are shown. (b) Structure model of alternately stacked graphene sheets and C60 monolayers, where C60 molecules can rotate between graphene sheets.
(a)(b)


## 4. Conclusion

At present, preliminary experiment indicates it is possible to intercalate huge fullerene molecules, such asC70 and La@C82 larger than a C60 molecule into graphite. Hence it is expected that the unique structure comprising huge fullerene molecules intercalated into graphite will give rise to attractive novel applications such as superlubrication materials, variable nanocapacitance, nanoswitches, and hydrogen storage in the future. Moreover, since the tribological test of grease and oils with an additive of this nanocomposite powder exhibits excellent lubricating performance with an ultralow friction previously unattained, the structure and material properties are expected to be more attractive also from scientific and material points of view. These are examples of the application that shows the novel mechanical property, and the intercalated materials will lead to promising materials with novel mechanical, physical, and electrical properties.



---

*Source: 891514-2010-08-25.xml*